Improving Thermal, Mechanical, and Barrier Properties of Feather Keratin/Polyvinyl Alcohol/Tris(hydroxymethyl)aminomethane Nanocomposite Films by ...
Page content transcription
If your browser does not render page correctly, please read the page content below
nanomaterials Article Improving Thermal, Mechanical, and Barrier Properties of Feather Keratin/Polyvinyl Alcohol/Tris(hydroxymethyl)aminomethane Nanocomposite Films by Incorporating Sodium Montmorillonite and TiO2 Shufang Wu 1 , Xunjun Chen 1, *, Minghao Yi 1 , Jianfang Ge 1 , Guoqiang Yin 1,2 , Xinming Li 1 and Ming He 1 1 Green Chemical Engineering Institute, Zhongkai University of Agriculture and Engineering, Guangzhou 510225, China; SFWu2018@163.com (S.W.); MHYi0848@163.com (M.Y.); email@example.com (J.G.); firstname.lastname@example.org (G.Y.); email@example.com (X.L.); firstname.lastname@example.org (M.H.) 2 Guangzhou Key Laboratory for Efficient Utilization of Agricultural Chemicals, Guangzhou 510225, China * Correspondence: email@example.com; Tel.: +86-020-3417-2870 Received: 18 January 2019; Accepted: 13 February 2019; Published: 20 February 2019 Abstract: In this study, feather keratin/polyvinyl alcohol/tris(hydroxymethyl)aminomethane (FK/PVA/Tris) bionanocomposite films containing two types of nanoparticles, namely one-dimensional sodium montmorillonite (MMT) clay platelets (0.5, 1, 3, and 5 wt%) and three-dimensional TiO2 nanospheres (0.5, 1, 3, and 5 wt%), are prepared using solvent casting method. X-ray diffraction studies confirm the completely exfoliated structure of FK/PVA/Tris/MMT nanocomposites. The successful formation of new hydrogen bonds between the hydroxyl groups of the film matrix and the nanofillers is confirmed by Fourier transform infrared spectroscopy. The tensile strength, elongation at break, and initial degradation temperature of the films are enhanced after MMT and TiO2 incorporation. The water vapor permeability, oxygen permeability, and light transmittance decrease with increase in TiO2 and MMT contents. In summary, nanoblending is an effective method to promote the application of FK/PVA/Tris blend films in the packaging field. Keywords: feather keratin; tris(hydroxymethyl)aminomethane; sodium montmorillonite; TiO2 ; solvent casting; nanocomposite 1. Introduction Environmental pollution and shortage of resources have forced researchers to explore biodegradable packaging materials as a replacement for petroleum-based synthetic plastics . However, biodegradable packaging has limitations in terms of heat resistance, water resistance, mechanical properties, and cost . At the same time, the use of edible starch or protein to prepare packaging materials may cause competition for food resources. Nonfood-borne keratin is a promising candidate for biodegradable packaging. Keratin is abundantly present in animal hair, feathers, and hooves (protein content 80–90%). In fact, feathers and hair are derivatives of keratinization of animal epidermal cells. It is estimated that the annual production of feathers, feather poles, and livestock slaughter (or its by-products) in the United States is approximately 3 to 4 billion tons  and that in China is more than 1.5 billion tons , most of which are treated as waste. This not only causes environmental pollution, but also wastage of resources. Keratin can be extracted from feathers by physical , chemical [6–8], or microbial methods [9,10], and keratin films can be prepared by casting [11–13], hot press forming , electrospinning [15–17], Nanomaterials 2019, 9, 298; doi:10.3390/nano9020298 www.mdpi.com/journal/nanomaterials
Nanomaterials 2019, 9, 298 2 of 17 etc. By using keratin films in the packaging field, “white pollution” can be reduced and the added value of keratin can be increased. The main disadvantage of biodegradable feather keratin (FK) film is that it is brittle and has poor toughness (in the absence of plasticizer). These properties can generally be improved by blending and cross-linking. From our previous research, we found that blending of FK, polyvinyl alcohol (PVA), and tris(hydroxymethyl)aminomethane (Tris) can improve the mechanical properties of FK-based films . However, the moisture sensitivity of the blend films is high, which limits their application in the packaging field. Cross-linking modification of FK-based film with CaCl2 , transglutaminase, and genipin can improve its water resistance and mechanical properties; however, the barrier properties of cross-linked films are not good, especially oxygen barrier properties . Therefore, other methods need to be explored to further improve the overall performance of FK-based films, especially mechanical, barrier, and thermal properties. The use of nanomaterials to modify biodegradable polymers is an important approach to improving the properties of biodegradable polymers. Compared with traditional composite materials, a low percentage of nanomaterials can considerably increase the mechanical strength of the polymer, reduce weight, increase heat resistance, and improve the barrier properties of food packaging materials to moisture, oxygen, carbon dioxide, ultraviolet radiation, and volatiles. Montmorillonite is the most commonly used one-dimensional layered silicate material owing to its environmental friendliness and low-cost . Abdallah et al.  used MMT which was prepared using spray freeze-drying (SFD-MMT) as reinforcement to prepare nanocomposites with poly(lactic acid) (PLA). It is shown that SFD-MMT provide satisfactory enhancements in rheological and mechanical properties of PLA. Song et al.  studied the effect of montmorillonite on the properties of keratin films. The results showed that the tensile strength of keratin nanocomposites increased with increase in the montmorillonite content (1–7%), and the water vapor permeability (WVP) reduced with increase in the montmorillonite content. Johannes Bott and Roland Franz  studied the migration potential of laponite in food. The authors claimed that the sample films with different loadings of laponite were stored for 10 days at 60 ◦ C, and no migration of laponite was found at a limit of detection of 22 µg laponite per Kg food. It can be concluded that the laponite (which represents the worst case of any larger structural type of clay) does not migrate into the food once it is incorporated into the polymer matrix. Titanium dioxide (TiO2 ) has been the most widely studied three-dimensional nanoparticle in the past decade, because it is an inert and inexpensive material. TiO2 exhibits antibacterial properties and can be used for active packaging of foods . It can also effectively inactivate antibiotic-resistant bacteria under ultraviolet irradiation , besides exhibiting photocatalytic activity. By blending the polymer with nano-TiO2 , the physical properties of the polymer can be improved , biodegradability of the synthetic polymer can be increased [27,28], and degradation of organic pollutants can be promoted [29,30]. Considering the excellent properties of MMT and TiO2 , nanoblending them with keratin will inevitably improve the physical performance of keratin films. To the best of our knowledge, studies on nanomodification of keratin with MMT and TiO2 are scarce. Therefore, in this study, MMT and TiO2 nanomodified FK/PVA/Tris blend films were prepared by the solution casting method, and the effects of their concentrations on the properties of FK/PVA/Tris blended films were investigated. 2. Materials and Methods 2.1. Materials PVA (analytical grade, degree of polymerization = 1700, degree of alcoholysis = 99) was supplied by Aladdin Ltd. (Shanghai, China). Tris was provided by Shanghai Ebene Chemical Reagent Co., Ltd. (China). TiO2 (content = 99.8%, anatase) was purchased from Aladdin Ltd. (Shanghai, China). The average diameter of TiO2 particles (as reported by the company) is approximately 60 nm. Sodium
Nanomaterials 2019, 9, 298 3 of 17 montmorillonite (MMT, content > 98%), was obtained from Mingsen Plastic Materials Co. Ltd. (Dongguan, China), and chicken FK powder was prepared as described in our previous work . Deionized (DI) water was employed as the solvent. 2.2. Preparation of 1% Nanoparticle Solutions Solutions of MMT and TiO2 were prepared by adding MMT or TiO2 powder (1 g) and Tris (3 g) to DI water (96 g) at 30 ◦ C with continuous stirring for 1 h, ultrasonication for 1 h (power ratio is 60%), and then continuous stirring for 24 h. 2.3. Preparation of the Nanocomposite Films Referring to our previous work , P-40-25 (FK to PVA weight ratio of 60:40 and a Tris content of 25 wt% relative to the total weight of FK and PVA) was selected as the control group. The procedure for preparation of the nanocomposite films is as follows. The extracted FK powder (1.2 g) and 6% PVA solution (13.33 g) were weighed in a beaker (the total solid mass of FK + PVA was set to 2 g), and a certain amount of 6% Tris solution and DI water were added with continuous stirring at 40 ◦ C for 30 min. Then, 1% of the nanoparticle solution consisting of 1, 2, 6, and 10 g (accounting for the total weight of FK and PVA 0.5%, 1%, 3% and 5%, respectively) was added with continuous stirring at 40 ◦ C for 1 h. The specific amounts of each substance added are shown in Table 1. The total mass of the final film forming solution was maintained at 50 g. The solution was ultrasonicated for 0.5 h (power ratio of 60%), followed by magnetic stirring in a constant temperature water bath at 40 ◦ C for 1 h. The cooled mixed solution was poured into polypropylene dishes (15 × 18 cm2 ). Nanomodified FK/PVA/Tris composite film was obtained by drying in a humidity chamber at 25 ◦ C and 50% relative humidity for 24 h. The different steps in the film forming process are shown in Figure 1. The blend films were named x-MMT and x-TiO2 , where x is the weight percentage of the nanoparticle relative to the total weight of FK and PVA in the film. The resulting blended films were conditioned at 25 ◦ C and 50% relative humidity for 48 h prior to testing. Table 1. Compositions of the different samples of blend films. FK Powder 6% PVA 6% Tris 1% MMT 1% TiO2 H2 O Sample (g) (g) (g) (g) (g) (g) P-40-25 1.2 13.33 8.33 0 0 27.17 0.5%-MMT 1.2 13.33 7.83 1 0 26.67 1%-MMT 1.2 13.33 7.33 2 0 26.17 3%-MMT 1.2 13.33 5.33 6 0 24.17 5%-MMT 1.2 13.33 3.33 10 0 22.17 0.5%-TiO2 1.2 13.33 7.83 0 1 26.67 1%-TiO2 1.2 13.33 7.33 0 2 26.17 3%-TiO2 1.2 13.33 5.33 0 6 24.17 5%-TiO2 1.2 13.33 3.33 0 10 22.17
Nanomaterials 2019, 9, 298 4 of 17 Nanomaterials 2019, 8, x FOR PEER REVIEW 4 of 17 Figure 1. Different steps in the film forming process. Figure 1. Different steps in the film forming process. 2.4. Characterization 2.4. Characterization The cross-sections (prepared by liquid nitrogen freezing) and the surface morphologies of the film samplesThewere cross‐sections observed by (prepared scanningby liquid microscopy electron nitrogen freezing)(SEM, EVO and 18;theCarl surface morphologies Zeiss, Jena, Germany) of the at film an samples were accelerating voltageobserved of 10 kV bytoscanning characterize electron microscopy the uniformity (SEM, EVO distribution. of nanoparticle 18; Carl Zeiss, Jena, Prior to Germany) the at an accelerating SEM observations, the samples voltage were of 10 kV coated with toa characterize fine gold layer the foruniformity 45 s. of nanoparticle distribution. Prior to the Fourier transform SEM observations, infrared spectroscopy the samples (FTIR) studies were coated of the film with samplesa fine gold were layer out carried for using 45 s. Fourier transform infrared spectroscopy (FTIR) studies of an infrared spectrometer (Spectrum 100, Perkin-Elmer, Fremont, CA, USA) in the attenuated total the film samples were carried out using an infrared reflectance spectrometer mode between 4000 and (Spectrum 650 cm 100, − 1 Perkin‐Elmer, (eight Fremont, CA, The scans per wavenumber). USA) in the MMT attenuated and the TiO2 total reflectance powders modebetween were tested between4000 4000and and 450 650 cm cm− −11(eight scans per wavenumber). The MMT and the (four scans per wavenumber) by tableting with TiO2 powders potassium were tested between 4000 and 450 cm−1 (four scans per wavenumber) by tableting with bromide. potassium bromide. of the sample was determined by powder X-ray diffraction (XRD, D-MAX 2200 The crystallinity VPC,The crystallinity RIGAKU Company of the sample Ltd., Tokyo, wasJapan) determined with Cu byKα powder X‐ray diffraction irradiation at an applied (XRD, D‐MAX voltage of 402200 kV VPC, RIGAKU Company Ltd., ◦ Tokyo, Japan) (30 mA), 2θ scan range of 3 to 80 , and a scan speed of 5 ·min . with Cu ◦ K − 1 irradiation at an applied voltage of 40 kV (30 mA), 2θ scan range ofanalysis Thermogravimetric 3 to 80,(TGA) and a was scancarried speed of out5·min using a. thermogravimetric analyzer (TGA2, −1 Thermogravimetric analysis (TGA) Mettler Toledo, Switzerland), and the mass of the sample was carried out using tested a thermogravimetric was 3–5 mg. Under analyzer (TGA2, the protection Mettler Toledo, Switzerland), and the mass of the − sample 1 tested was of N2 , the gas flow rate was maintained at 50 ml·min . The temperature range of the test was 40 to 35 mg. Under the protection of 700 ◦ N2, the gas flow C, and rate was the heating maintained rate was 10 Cat ◦ ·min − 50 ml·min 1 . −1. The temperature range of the test was 40 to 700 C, and the heating rate was 10 C·min −1. The tensile properties of the film samples were measured using a microcomputer-controlled The tensile electronic universalproperties of the film testing machine samples (CMT6503, were measured Shenzhen MTS Testusing Machine a microcomputer‐controlled Company Ltd., Shenzhen, electronic China), universal according testing to the ASTM machine (CMT6503, D 882 standard, at aShenzhen speed of MTS 10 mmTest −1 and a fixture ·minMachine Company Ltd., distance Shenzhen, China), according to the ASTM D 882 standard, at of 40 mm. The films were cut into samples measuring 75 mm × 10 mm, and the sample thicknesses a speed of 10 mm·min −1 and a fixture distance were of 40 mm. measured usingThe films external a digital were cutmicrometer into samples measuring (accurate to 0.00175 mm mm).× The10 mm, and the sample measurements were thicknesses were measured using a conducted in triplicate and average values calculated. digital external micrometer (accurate to 0.001 mm). The measurements were conducted in triplicate and average values The WVP values of the films were measured using a water vapor transmittance tester (W3/030,calculated. The WVP Labthink valuesChina). Ltd., Jinan, of the First, films all werethemeasured film samples usingwere a water cut into vapor transmittance circular shapes with tester (W3/030, diameters of Labthink Ltd., Jinan, China). First, all the film samples were cut into 3 cm and were filled into the instrument. Then, the test conditions were set as follows; temperature: circular shapes with diameters of ◦3C,cm 38 and were relative humidityfilledacross into the the film: instrument. Then, the time: 90–0%, warm-up test conditions were setinterval: 4 h, and weighing as follows; 2 h. temperature: The measurements 38 C,wererelative humidity conducted across the in triplicate andfilm: average900%,values warm‐up calculated.time: 4 h, and weighing interval: The 2oxygen h. Thepermeability measurements (OP)were conducted values in triplicate of the films and average were measured values using calculated. an oxygen permeability testerThe oxygen permeability (VAC-VBS, Labthink Ltd., (OP) values Jinan, of theaccording China) films weretomeasured the GB/Tusing an oxygen 1038-2000 permeability standard. Firstly, tester (VAC‐VBS, Labthink Ltd., Jinan, China) according to the GB/T the samples were cut into circular shapes with diameters of 5.5 cm and placed in the instrument. Then, 1038‐2000 standard. Firstly, the samples were cut into circular shapes with diameters of 5.5 cm and placed in the instrument. Then, Nanomaterials 2019, 8, x; doi: FOR PEER REVIEW www.mdpi.com/journal/nanomaterials
Nanomaterials 2019, 9, 298 5 of 17 Nanomaterials 2019, 8, x FOR PEER REVIEW 5 of 17 the test the test conditions conditions were were setset as as test test gas gas pressure: pressure: 1.01 1.01 ××10 105Pa 5 Paand andupper upperand andlower lowerdegassing degassing time: 4 time: h. The measurements were conducted in triplicate and average values 4 h. The measurements were conducted in triplicate and average values calculated. calculated. The transmittance The transmittance of of the the films films in in the the wavelength wavelength range range from from 200 200 to to 800 800 nm nm was was measured measured using using a spectrophotometer (UV‐1800, Shimadzu Corporation, Chengdu, China) a spectrophotometer (UV-1800, Shimadzu Corporation, Chengdu, China) according to the method according to the method described by described byHe Heetetal.al. . . TheThe filmfilm samplesample wasinto was cut cutrectangular into rectangular pieces pieces (10 × 40(10 mm× 240 mm ) and 2) and directly directly attached attached to the Empty to the cuvette. cuvette.cuvettes Empty were cuvettes usedwere used controls. as blank as blank The controls. The transparency transparency value (T) ofvalue the (T) of the films was calculated using the films was calculated using the following equation. following equation. T= − (log T600)/ T = −(log T600 )/x where T600 is the transmittance at 600 nm and x is the film thickness (mm). The measurements were conducted where T600 in triplicate is the and average transmittance at 600values nm andcalculated. x is the film thickness (mm). The measurements were conducted in triplicate and average values calculated. 3. Results and Discussion 3. Results and Discussion 3.1. Morphology of the Nanocomposite Films 3.1. Morphology of the Nanocomposite Films Upon visual observation, all the nanocomposite films exhibited smooth surfaces with no Uponpores obvious visual observation, (see Supplementary all the nanocomposite Materials Image films exhibited S1). The smooth surfaces with appearance of no theobvious MMT pores (see Supplementary Materials Image S1). The appearance of the nanocomposite films was similar to that of the control film P‐40‐25: yellowish in color and optically MMT nanocomposite films was similar to that of the control film P-40-25: yellowish in color transparent. However, with the addition of TiO2, the films gradually whitened and the light and optically transparent. However, with the addition transmittance of TiO2 , This decreased. the films gradually is because TiOwhitened 2 is a white and the light coloring transmittance agent and has adecreased. This is strong scattering because TiO is a effect on light [26,31]. 2 white coloring agent and has a strong scattering effect on light [26,31]. To To elucidate elucidate thethe influence influence of of the the addition addition of of nanomaterials nanomaterials on on the the microstructure microstructure and and the the uniformity uniformity of of the theblend blendfilms,films,the the surface surface andand thethe cross-section cross‐section of 1%-MMT, of 1%‐MMT, 5%-MMT, 5%‐MMT, 1%‐TiO1%-TiO2, and2, and 5%-TiO nanocomposite 5%‐TiO2 nanocomposite 2 films were analyzed by SEM, and the results are films were analyzed by SEM, and the results are shown in Figure 2. All theshown in Figure 2. All the blendblendfilmsfilms exhibit exhibit a rough a rough surface surface withwith granular granular protrusions, protrusions, andand more more granules granules areare observed observed in in the film matrix with increase in the content of MMT and TiO the film matrix with increase in the content of MMT and TiO2. These granular protrusions are 2 . These granular protrusions are evenly evenly distributed distributedononthethe surface surfaceof the of blend film, and the blend film,noandlargenoaggregates of particles large aggregates of were observed, particles were indicating that the nanoparticles observed, indicating are uniformly that the nanoparticles disperseddispersed are uniformly in the film matrix. in the The analysis film matrix. of the The analysis cross-section of the cross‐sectioncan better indicate can better the dispersion indicate uniformity the dispersion of theofnanoparticles uniformity in theinblend the nanoparticles the blendfilm. As evident from the cross-sectional structure of the blend films, the addition film. As evident from the cross‐sectional structure of the blend films, the addition of nanoparticles of nanoparticles roughened the cross-section, roughened and small particles the cross‐section, and small areparticles embedded are in the film matrix. embedded Withmatrix. in the film increaseWithin the content increase in of nanoparticles, more particles are observed along the side of the cross-section the content of nanoparticles, more particles are observed along the side of the cross‐section (e.g., left (e.g., left side of the sidecross-sectional SEM image of the cross‐sectional SEM of 5%-TiO image 2ofsample), 5%‐TiOwhich2 sample),may which be attributed may be to attributed the deposition to the of nanoparticles deposition of during the film during nanoparticles formation theprocess. The moreprocess. film formation the amount The ofmore nanoparticles the amount added, of the more significant is the deposition, resulting in uneven distribution nanoparticles added, the more significant is the deposition, resulting in uneven distribution of the of the nanoparticles in the cross-section nanoparticlesofinthe theblend film. cross‐section of the blend film. Figure 2. Cont. Nanomaterials 2019, 8, x; doi: FOR PEER REVIEW www.mdpi.com/journal/nanomaterials
Nanomaterials 2019, 9, 298 6 of 17 Nanomaterials 2019, 8, x FOR PEER REVIEW 6 of 17 Figure 2. Representative SEM images of the surface morphology (left; 2000X) and the fracture Figure 2. Representative morphology (right; 3000X)SEM of theimages of the surface morphology (left; 2000X) and the fracture blend films. morphology (right; 3000X) of the blend films. 3.2. FTIR Analysis 3.2. FTIR Analysis Figure 3a shows the FTIR spectra of pure MMT and TiO2 in the wavelength range of Figure 4000–450 −1 . In cm3(a) shows the FTIR the case of MMT, spectra of pure the peaks MMT and observed TiO2 in3441.56, at 3625.24, the wavelength and 1087.76 rangecm− of1 4000450 correspond cmto‐1.the In MMT the case of MMT,stretching surface-OH the peaks observed vibration, MMTat 3625.24, 3441.56, interlayer-OH and 1087.76 stretching cm‐1 vibration, correspond and silicon bondto theinMMT MMTsurface‐OH structure , stretching vibration, respectively. In the MMT interlayer‐OH FTIR spectrum of TiOstretching 2 , the peaksvibration, at 3413.5, and silicon 1614.23, andbond in MMT 1000–450 cm−structure 1 correspond ,torespectively. -OH stretching In the FTIR spectrum vibration of TiO2,-OH of TiO2 surface, the peaks bending at 3413.5, vibration,1614.23, and 1000450 and Ti-O-Ti stretchingcm ‐1 correspond vibration to ‐OH stretching vibration of TiO2 surface, ‐OH , respectively. bending vibration, To fully and Ti‐O‐Ti understand stretchingbetween the interaction vibrationthe, respectively. FK/PVA/Tris blend film and the nanoparticles, To fully the FTIR understand spectra of differentthe nanomodified interaction between the FK/PVA/Tris FK/PVA/Tris blend blend films werefilm and the nanoparticles, investigated (Figure 3b,c). the The FTIR infraredspectra spectra of of different the blend nanomodified films changed FK/PVA/Tris significantlyblend films were investigated after nanomodification and the(Figs. peak 3(b)(c)). positions The infrared shifted. When spectra 5%-MMT of the blend was addedfilms to changed the blendsignificantly film, the FTIR after nanomodification peaks of the control film and the peak P-40-25 positions at 3327.68,shifted. 2929.28,When 5%‐MMT 1535.82, and 1039.83 cm−1 (corresponding was added to the blend film,to O–HtheandFTIRN–H peaks of the association, control –CH film P‐40‐25 stretching  amide vibration, at 3327.68, 2929.28, II band, and C–O1535.82, and 1039.83 stretching cmrespectively) vibration, ‐1 (corresponding shiftedto to O–H and 3289.95, N–H association, –CH stretching vibration, amide II band, and C–O stretching vibration, respectively) shifted to 3289.95, 2921.14, 1539.95, and 1021.83 cm‐1, respectively. At the same time, Nanomaterials 2019, 8, x; doi: FOR PEER REVIEW www.mdpi.com/journal/nanomaterials
Nanomaterials 2019, 9, 298 7 of 17 Nanomaterials 2019, 8, x FOR PEER REVIEW 7 of 17 2921.14, 1539.95, and 1021.83 cm−1 , respectively. At the same time, the absorption peaks of MMT the3625.24 at absorption peakscmof and 3441.56 −1 MMT at 3625.24 disappeared; this is and 3441.56 because cm‐1 disappeared; MMT-dispersed this isexfoliated films exhibited because MMT‐dispersed films nanomorphology exhibited using (as confirmed exfoliated XRD),nanomorphology and the hydroxyl(as confirmed groups between usingthe XRD), andand interlayer the hydroxyl the surfacegroups of the between layer were theaffected. interlayer and 5%-TiO When the surface 2 wasof the added layer to were the affected. blend film, When the 5%‐TiO absorption 2 was added peaks to the of P-40-25 blend  film, the at 3327.68, absorption 1633.82, peaks 1237.65, andof P‐40‐25 1039.83 −1 (corresponding cm at 3327.68, 1633.82, to O–H1237.65, and and N–H 1039.83 cm‐1amide association, (corresponding I band, amideto O–H and N–H III band, association, and C–O stretchingamide I band, vibration) amidetoIII shifted band, 16410.11, 3289.03, and C–O stretching 1217.44, andvibration) 1030.36 cm −1 , respectively, shifted to 3289.03,and 16410.11, 1217.44,peak the absorption and of1030.36 TiO2 atcm cm−1 disappeared. ‐1, respectively, 3413.5 and the absorption These peak changes in of theTiO 2 atspectrum FTIR 3413.5 cmindicate ‐1 disappeared. These changes the formation of stronginhydrogen the FTIR bonding spectrumbetween indicate the the formation of strong nanoparticles and thehydrogen film matrixbonding . between the nanoparticles and the film matrix . TiO2 powder (a) P-40-25 3441.56 (b) 1614.23 2929.28 1237.65 1132.21 3273.68 1633.82 1039.83 0.5%-MMT 1535.82 3413.5 1067.68 Transmittance (%) Transmittance (%) 1%-MMT MMT powder 3%-MMT 1635.07 5%-MMT 3441.56 1455.31 796.65 3625.24 3289.95 2921.14 1539.95 1087.76 1020.02 4000 3500 3000 2500 2000 1500 1000 500 4000 3500 3000 2500 2000 1500 1000 -1 -1 Wavenumber (cm ) Wavenumber (cm ) P-40-25 (c) 3413.5 2929.28 1237.65 1039.83 0.5%-TiO2 3273.68 1633.82 1535.82 Transmittance (%) 1%-TiO2 3%-TiO2 5%-TiO2 1217.44 3289.03 1641.01 1030.36 4000 3500 3000 2500 2000 1500 1000 -1 Wavenumber (cm ) Figure 3.3. FTIR Figure FTIR spectra spectra of of (a) (a) MMT MMT powder powder and and TiO TiO22 powder, (b) (b) P-40-25 P‐40‐25 incorporated incorporated with MMT, and (c) and (c) P-40-25 P‐40‐25incorporated incorporatedwith withTiO TiO22.. 3.3. XRD Studies 3.3. XRD Studies To study the dispersion properties of the nanoparticles in the film matrix, XRD analyses of To study the dispersion properties of the nanoparticles in the film matrix, XRD analyses of pure MMT, TiO2 powders, and blend films were carried out. Figure 4a shows the XRD pattern of pure MMT, TiO2 powders, and blend films were carried out. Figure 4(a) shows the XRD pattern of MMT powder and FK/PVA/Tris nanocomposite films incorporated with different concentrations of MMT powder and FK/PVA/Tris nanocomposite films incorporated with different concentrations of MMT. For pure MMT, the characteristic diffraction peak appears at 2θ = 7.07◦ , and the layer spacing MMT. For pure MMT, the characteristic diffraction peak appears at 2θ = 7.07°, and the layer spacing corresponding to d001 , as calculated using Bragg’s law, is 1.249 nm . For the MMT nanocomposite corresponding to d001, as calculated using Bragg’s law, is 1.249 nm . For the MMT film, the peak at 7.07◦ disappeared. This result indicates an exfoliated nanomorphology, suggesting nanocomposite film, the peak at 7.07° disappeared. This result indicates an exfoliated that the molecular chains of FK, PVA, and Tris entered into the gallery space of the silicate layers. nanomorphology, suggesting that the molecular chains of FK, PVA, and Tris entered into the Exfoliation and dispersion of MMT nanoplatelets may be due to strong interactions between FK, PVA, gallery space of the silicate layers. Exfoliation and dispersion of MMT nanoplatelets may be due to Tris, and MMT , as confirmed by FTIR studies. The hydroxyl groups of FK, PVA, and Tris can strong interactions between FK, PVA, Tris, and MMT , as confirmed by FTIR studies. The directly hydroxyl interact groupswith the sodium of FK, PVA, and ionsTris of the canMMT gallery directly (similar interact withtothe water molecules) sodium ions oforthe with the MMT edge gallery (similar to water molecules) or with the edge hydroxyl groups of the MMT layers, and the hydroxyl groups of the MMT layers, and the amino groups of FK and Tris can interact with the hydroxyl groups amino groups of of FKthe andMMTTris surface, forming can interact withathe very compatible hydroxyl system. groups AliMMT of the et al. surface,  reported thata forming very compatible system. Ali et al.  reported that MMT (addition amount < 10%) was present in Nanomaterials 2019, 8, x; doi: FOR PEER REVIEW www.mdpi.com/journal/nanomaterials
peak position shifted to the low wave number and moved to 25.1° of 5%‐TiO2. If there is no interaction between TiO2 and the film matrix, a simple superposition according to the ratio of these materials can be observed in the XRD pattern of the quaternary nanocomposite film, but the peak intensity of the quaternary nanocomposite changes and the peak position moved, it can be judged that there is an interaction force between them, which is consistent with the FTIR spectrum analysis. Nanomaterials 2019, 9, 298 8 of 17 Similar X‐ray diffraction patterns were observed in all nanocomposite films with different MMT or TiO2 concentrations, since the main substrates of the film were FK, PVA, and Tris. At the same time, MMT it canamount (addition be seen
Nanomaterials 2019, 9, 298 9 of 17 Nanomaterials 2019, 8, x FOR PEER REVIEW 9 of 17 the blend films. Thus, the nanocomposite films can reach the same amount of water vapor evaporation loss at astage, second higherthetemperature. Tonset of theInnanocomposite the second stage, thewas film Tonset of the nanocomposite significantly improved,film was significantly compared with that improved, ◦ of P‐40‐25; compared the increase with wasthat of P-40-25; ~1421 °C. In the increase addition, was Tmax ~14–21 slightly, improved C. In addition, and theTmax finalimproved residual slightly, and the final residual amount increased. These data indicate that the addition amount increased. These data indicate that the addition of nanoparticles can improve the thermal of nanoparticles can improve stability of thetheFK/PVA/Tris thermal stability blendoffilm the owing FK/PVA/Tris blend to the high film owing thermal to the stability highnanoparticles of the thermal stability and of the the nanoparticles barrier andnanoparticles. effect of the the barrier effect of the nanoparticles. Nanoparticles can form Nanoparticles can form a protective physical a protective barrier on the physical surface of barrier on the surface the material, whichofprevents the material, volatilewhich prevents volatile degradation products degradation products from escaping fromfrom the escaping from composite andthe composite ultimately and ultimately retards retards the degradation ofthe thedegradation of the composite [38,39]. composite [38,39]. 100 100 (a) (b) 0.5%-MMT 0.5%-TiO2 1%-MMT 1%-TiO2 3%-MMT 80 5%-MMT 80 3%-TiO2 P-40-25 5%-TiO2 P-40-25 60 Weight (%) 60 Weight (%) 40 40 20 20 0 0 100 200 300 400 500 600 700 100 200 300 400 500 600 700 Temperature (℃) Temperature (℃) Figure 5.5.Thermogravimetric Thermogravimetric curves curves of (a)ofP-40-25 (a) P‐40‐25 incorporated incorporated with with MMT and MMT and incorporated (b) P-40-25 (b) P‐40‐25 incorporated with TiO2 . with TiO2. Table 2. Table Thermogravimetric analysis 2. Thermogravimetric analysis (TGA) (TGA) results results of of P-40-25 P‐40‐25 incorporated incorporated with with MMT MMT and and TiO TiO22.. ∆1 1 ∆2 Sample Residue (%) Sample Td1 (◦ C) (◦ C) ◦ Residue (%) Td1 (C) TT onset onset (C) TmaxTmax (C)( C) P-40-25 P‐40‐25 214.83 214.83 167.5 329.33 167.5 329.33 8.75 8.75 0.5%-MMT 231.83 199.17 330.67 8.86 0.5%‐MMT 1%-MMT 231.83 235.83 199.17 330.67 202.17 330.83 8.8610.07 3%-MMT 1%‐MMT 230.17 235.83 200.5 330.17 202.17 330.83 10.0710.55 5%-MMT 230 202.33 329.67 12.11 3%‐MMT 230.17 200.5 330.17 10.55 0.5%-TiO2 229.67 199.67 330.17 9.29 5%‐MMT 1%-TiO 2 230 234.5 202.33 329.67 204331 12.119.23 3%-TiO 0.5%‐TiO 2 236.5 229.67 2 201.83 331.33 199.67 330.17 9.2911.44 5%-TiO2 227.5 196.17 330 10.64 1%‐TiO2 204 234.5 331 9.23 3%‐TiO2 201.83 236.5 331.33 11.44 3.5. Mechanical Properties 5%‐TiO2 196.17 227.5 330 10.64 Figure 6 shows the stress–strain relationship of the control film and the nanocomposite films. It isMechanical 3.5. evident that the addition of nanoparticles improves the mechanical properties, i.e., both the Properties elongation at break and the tensile strength of the FK/PVA/Tris blend films. Figure 7 shows the Figure 6 shows the stress–strain relationship of the control film and the nanocomposite films. It elastic modulus, tensile strength, and elongation at break of the FK/PVA/Tris blend films prepared is evident that the addition of nanoparticles improves the mechanical properties, i.e., both the with different contents of MMT and TiO2 . Tensile properties for P-40-25 were from Chen et al. . elongation at break and the tensile strength of the FK/PVA/Tris blend films. Figure 7 shows the The specific mechanical properties of the nanocomposite films can be found in the Supplementary elastic modulus, tensile strength, and elongation at break of the FK/PVA/Tris blend films prepared Materials (Table S1). The elastic modulus of P-40-25 reduced from 416.78 MPa to 339.85 (5%-MMT) and with different contents of MMT and TiO2. Tensile properties for P‐40‐25 were from Chen et al. . 280.38 MPa (5%-TiO2 ); the elongation at break of P-40-25 increased from 10.83% to 22.07 (5%-MMT) The specific mechanical properties of the nanocomposite films can be found in the Supplementary and 47.9% (5%-TiO2 ); and the tensile strength of P-40-25 increased from 9.58 MPa to 10.25 (5%-MMT) Materials (Table S1). The elastic modulus of P‐40‐25 reduced from 416.78 MPa to 339.85 (5%‐MMT) and 13.12 MPa (5%-TiO2 ). It is worth noting that the two different nanoparticles imparted different and 280.38 MPa (5%‐TiO2); the elongation at break of P‐40‐25 increased from 10.83% to 22.07 effects on the mechanical properties of the FK/PVA/Tris blend films, and these mechanical properties (5%‐MMT) and 47.9% (5%‐TiO2); and the tensile strength of P‐40‐25 increased from 9.58 MPa to varied at different concentrations of the various nanoparticles. 10.25 (5%‐MMT) and 13.12 MPa (5%‐TiO2). It is worth noting that the two different nanoparticles imparted different effects on the mechanical properties of the FK/PVA/Tris blend films, and these mechanical properties varied at different concentrations of the various nanoparticles. Nanomaterials 2019, 8, x; doi: FOR PEER REVIEW www.mdpi.com/journal/nanomaterials
Thus, nano‐TiO2 is more effective than MMT in improving the mechanical properties of the blend films. This may be related to the compatibility and the dispersion uniformity of the nanoparticles with the film matrix. The water solubility of TiO2 is better than that of MMT, and the dispersion of TiO2 in the film matrix is more uniform; hence, the mechanical properties of the TiO2 nanocomposite Nanomaterials 2019, films 9, 298 are better than those of MMT nanocomposite films at the same concentration 10 of 17 of nanoparticles. (a) 12 (b) 10 10 8 8 Stress (MPa) Stress (MPa) 6 6 4 4 P-40-25 0.5%-TiO2 P-40-25 2 0.5%-MMT 1%-TiO2 2 1%-MMT 3%-TiO2 3%-MMT 5%-TiO2 0 5%-MMT 0 0 10 20 30 40 50 0 5 10 15 20 25 Strain (%) Strain (%) Figure Figure 6.6.Tensile Tensileproperties propertiesof of (a)(a) P‐40‐25 incorporated P-40-25 withwith incorporated MMT and and MMT (b) P‐40‐25 incorporated (b) P-40-25 with incorporated Nanomaterials with2. TiO2019, TiO . 8, x FOR PEER REVIEW 11 of 17 2 440 440 (a) 10.8 Elastic modulus (MPa) 28 (b) Elastic modulus (MPa) 50 13 Elongation at break (%) Elongation at break (%) 420 420 Tensile strength (MPa) 26 10.6 Tensile strength (MPa) 400 24 10.4 400 40 12 22 10.2 380 380 20 10.0 360 360 30 11 18 9.8 340 340 16 9.6 20 320 320 14 10 Nanomaterials 2019, 8, x; doi: FOR PEER REVIEW 9.4 www.mdpi.com/journal/nanomaterials 300 12 300 9.2 10 10 280 280 9.0 9 0 1 2 3 4 5 0 1 2 3 4 5 MMT content (%) TiO2 content (%) Figure 7. Tensile properties of (a) P-40-25 incorporated with MMT and (b) P-40-25 incorporated Figure with TiO27.. Tensile properties of (a) P‐40‐25 incorporated with MMT and (b) P‐40‐25 incorporated with TiO2. In the MMT nanocomposite film (Figure 7a), the elongation at break and the tensile strength of the 3.6. Barrier MMT nanoblendProperties of theincreased film first Blend Films and then decreased with increase in the MMT content, whereas the elastic modulus first decreased and then increased. This is attributed to the physical adsorption Barrier performance is a measure of the resistance of packaging materials to the scent of the and hydrogen bonding force between the MMT and the film matrix. When the MMT content is ≤3%, package as well as intrusion of gases, bacteria, etc. present outside the package. Materials with good MMT is uniformly dispersed into the film matrix owing to the exfoliated structure, and the interfacial barrier properties ensure the stability of the packaged product and extend its shelf life. Therefore, interaction between the film matrix and MMT enhances with increase in the MMT content. This results the barrier properties of packaging materials seriously affect their use in the field of packaging. The in better transfer of load or force from the film matrix to the nanoclay filler, while not easily breaking following sections describe the WVP, oxygen permeability, and UV barrier properties of the blend the film matrix–nanoclay interface during tensile deformation. With increase in the MMT content films. to 5%, MMT begins to aggregate, reducing the interfacial interaction between the film matrix and the nanoclay 3.6.1. WVP filler, thereby resulting in interfacial failure and decrease in the tensile strength and the elongation at break. Similar results were observed in tilapia skin gelatin/MMT blend films by NagarajanThe effects of the two nanoparticles on the WVP values of P‐40‐25 are shown in Figure 8. Figure et al. . 8(a)Inshows the case of TiO2values the WVP of P‐40‐25film nanocomposite incorporated (Figure 7b),with the different elongation contents at breakofand MMT. With increase the tensile strengthin ofthe theMMTTiO2 content, nanoblend the WVP value of the film increased with films decreased increase in the first TiOand then increased slightly. When the 2 content, and the elastic modulus MMT content is 3%, the WVP of the nanocomposite decreased. A possible reason is that when the film substrate is subjected film reaches a to minimum of 2.42 an external force,× it10is −12 g·cm easy −1·s ·Pa the −1 to excite −1, which is 21.68% surrounding lower matrix to than that microcracks generate of P‐40‐25 .andThis absorbmay be attributed energy because ofto the the stress strong interaction of MMT with the film matrix, which reduces the free volume concentration effect of the rigid TiO2 nanoparticles. At the same time, the existence of rigid particles of the film matrix and interferes with the transport of water vapor through the film matrix, hinders and inactivates crack propagation in the matrix, preventing destructive cracking, thereby extending the path of water vapor diffusion resulting in enhanced through the film toughness matrix . . reason Another In addition, is thatLiTiO et al.  pointed out that MMT as a 2 can strengthen the association of physical cross‐linking site can enhance the stability O–Ti–O bonds between the film matrix and the nanoparticles through of the network. Theelectrostatic strong interaction between attraction and hydrogen bonding, thereby forming a stable three-dimensional polymer matrix and improvingwater the film matrix and the MMT sheet consumes some hydrophilic groups, which decreases the the absorbed by capillary action at the interface, elongation and the tensile strength of the blend films [31,42]. thereby hindering the diffusion of water molecules. When the MMT content was increased to 5%, the WVP of the blend film increased slightly, but it was still smaller than that of the control film. This may be caused by the accumulation of MMT in the film matrix, which affects the water vapor barrier performance of the composite film. Similar results have been reported in the literature; for example, the addition of MMT was found to improve the water vapor barrier properties of fish gelatin film [40,45], chicken feather protein film , and starch/PVA composite film .
Nanomaterials 2019, 9, 298 11 of 17 Comparing the data in Figure 7, at the same content of nanoparticles, the mechanical properties of the TiO2 nanocomposite films are better than those of the MMT nanocomposite films. Thus, nano-TiO2 is more effective than MMT in improving the mechanical properties of the blend films. This may be related to the compatibility and the dispersion uniformity of the nanoparticles with the film matrix. The water solubility of TiO2 is better than that of MMT, and the dispersion of TiO2 in the film matrix is more uniform; hence, the mechanical properties of the TiO2 nanocomposite films are better than those of MMT nanocomposite films at the same concentration of nanoparticles. 3.6. Barrier Properties of the Blend Films Barrier performance is a measure of the resistance of packaging materials to the scent of the package as well as intrusion of gases, bacteria, etc. present outside the package. Materials with good barrier properties ensure the stability of the packaged product and extend its shelf life. Therefore, the barrier 2019, Nanomaterials properties of packaging 8, x FOR PEER REVIEW materials seriously affect their use in the field of packaging. 12 of 17 The following sections describe the WVP, oxygen permeability, and UV barrier properties of the blendTherefore, films. the water vapor barrier properties of the blend films of MMT and TiO2 nanoparticles are better than that of the control film. In particular, the water vapor resistance of 3.6.1. WVP film is superior to that of MMT blend film. TiO2 blend The effects of the two nanoparticles on the WVP values of P-40-25 are shown in Figure 8. FigureOxygen 3.6.2. 8a shows Permeability the WVP values of P-40-25 incorporated with different contents of MMT. With increase in the MMT The oxygen permeability content,(OP) the values WVP value of the of P‐40‐25 films decreased incorporated first and with different then increased contents of MMT slightly. When the are also shown MMT content in Figure 8(a). Theis OP3%,value the WVP of film of the the nanocomposite decreased first and film then reaches a minimum increased of slightly 2.42 × 10 −12 g·cm−1 ·s−1 ·Pa−1 , which is 21.68% lower than that of P-40-25 . This may be attributed with increase in the MMT content, a trend consistent with that of WVP. When the MMT content is to 3%,the strong the OP of interaction of MMT with the nanocomposite filmthereaches film matrix, which reduces a minimum of 2.521the free × 10 volume −5 cm 3·m−2·d of−1the ·Pa−1film matrix , which is and 78.6% interferes lower than withthattheoftransport of water vapor through the film matrix, extending the path of water P‐40‐25 . vaporThe diffusion OP value through the film of P‐40‐25 matrix . incorporated withIndifferent addition,contents Li et al.of TiOpointed 2 is shown outin that Fig.MMT 8(b). as The a physical cross-linking site can enhance the stability of the network. The oxygen barrier properties of the blend films decreased with increase in the TiO2 content. When the strong interaction between the TiOfilm matrixisand 2 content 5%,thetheMMT OPsheet of theconsumes some hydrophilic nanocomposite groups, film reaches which decreases a minimum of 7.355 the ×water 10−5 absorbed by capillary action at the interface, thereby cm ·m ·d ·Pa , which is 37.56% lower than that of P‐40‐25 . 3 −2 −1 −1 hindering the diffusion of water molecules. When the MMT content was The addition increased of MMT and TiOto 5%, the WVP of the 2 nanoparticles blend film improves the increased oxygen barrier slightly, but it was properties of still the smaller than that of the control film. This may be caused by the accumulation blend films because of the strong interaction between the nanoparticles and the film matrix; of MMT in the film matrix, small‐sized which affects the water nanoparticles have vapor a higherbarrier performance occupation of theofporous the composite film matrix.film.TheSimilar results filling up ofhavethe been voidsreported reduces the in the freeliterature; volume offor theexample, film matrix the and addition of MMT interferes withwas found to improve the transport of oxygenthe water through vapor the film barrier matrix,properties extending of the fishpath gelatin film [40,45], of diffusion chickenthrough of oxygen feather protein the filmfilm ,thereby matrix, and starch/PVA reducing composite the amountfilm . permeation . of oxygen 3.2 (a) 13 (b) 3.2 12 12 3.0 10 OP (×10 cm /(m ·d·Pa)) OP (×10 cm /(m ·d·Pa)) g/(cm·s·Pa)) g/(cm·s·Pa)) 3.0 11 8 2.8 2 2 10 2.8 3 3 6 -12 -12 9 WVP (×10 WVP (×10 -5 -5 2.6 2.6 4 8 2.4 2 7 2.4 0 6 0 1 2 3 4 5 0 1 2 3 4 5 MMT content (%) TiO2 content (%) Figure 8. 8. Water Water vapor vapor permeability permeability (WVP) (WVP) and and oxygen permeability permeability (OP) values of (a) P-40-25 P‐40‐25 P‐40‐25 incorporated with incorporated with MMT and (b) P-40-25 with TiO TiO22. 3.6.3. Light Transmission and Transparency Table 3 shows the values of transmittance of the MMT and the TiO2 nanomodified FK/PVA/Tris blend films at selected wavelengths in the range of 200 to 800 nm. With the addition of nanoparticles, the transmittance of the blend film decreased at all wavelengths, and the degree of reduction varied depending on the type and the content of the nanoparticles. When the content of nanoparticles is the same, the blend film with TiO2 has a smaller transmittance than that with MMT,
Nanomaterials 2019, 9, 298 12 of 17 Figure 8b shows the WVP values of P-40-25 incorporated with different contents of TiO2 . The WVP value of the films decreased with increase in the TiO2 content. When the TiO2 content is 5%, the WVP of the nanocomposite film reaches a minimum of 2.26 × 10−12 g·cm−1 ·s−1 ·Pa−1 , which is 26.86% lower than that of P-40-25 . The possible reason is the lower water solubility and hydrophilicity of TiO2 compared with those of keratin, PVA, and Tris, which blocks micro- and nanopathways in network structures . In addition, Zhou et al.  have reported that TiO2 has a hydrophobic coating effect on the surface of the film, which slows down the adsorption rate and reduces the WVP. Therefore, the water vapor barrier properties of the blend films of MMT and TiO2 nanoparticles are better than that of the control film. In particular, the water vapor resistance of TiO2 blend film is superior to that of MMT blend film. 3.6.2. Oxygen Permeability The oxygen permeability (OP) values of P-40-25 incorporated with different contents of MMT are also shown in Figure 8a. The OP value of the film decreased first and then increased slightly with increase in the MMT content, a trend consistent with that of WVP. When the MMT content is 3%, the OP of the nanocomposite film reaches a minimum of 2.521 × 10−5 cm3 ·m−2 ·d−1 ·Pa−1 , which is 78.6% lower than that of P-40-25 . The OP value of P-40-25 incorporated with different contents of TiO2 is shown in Figure 8b. The oxygen barrier properties of the blend films decreased with increase in the TiO2 content. When the TiO2 content is 5%, the OP of the nanocomposite film reaches a minimum of 7.355 × 10−5 cm3 ·m−2 ·d−1 ·Pa−1 , which is 37.56% lower than that of P-40-25 . The addition of MMT and TiO2 nanoparticles improves the oxygen barrier properties of the blend films because of the strong interaction between the nanoparticles and the film matrix; small-sized nanoparticles have a higher occupation of the porous film matrix. The filling up of the voids reduces the free volume of the film matrix and interferes with the transport of oxygen through the film matrix, extending the path of diffusion of oxygen through the film matrix, thereby reducing the amount of oxygen permeation . 3.6.3. Light Transmission and Transparency Table 3 shows the values of transmittance of the MMT and the TiO2 nanomodified FK/PVA/Tris blend films at selected wavelengths in the range of 200 to 800 nm. With the addition of nanoparticles, the transmittance of the blend film decreased at all wavelengths, and the degree of reduction varied depending on the type and the content of the nanoparticles. When the content of nanoparticles is the same, the blend film with TiO2 has a smaller transmittance than that with MMT, indicating that the TiO2 nanocomposite film has higher barrier light transmission performance than the MMT nanocomposite film. This is because TiO2 is a semiconductor and absorbs photon energy to excite electrons from the valence band to the conduction band, resulting in enhanced absorbance of the TiO2 film and reduced light transmission . Meanwhile, the light transmittance of the FK/PVA/Tris blend film decreased with increase in the nanoparticle content, which may be caused by light scattering effect of the nanoparticles distributed in the blended film matrix. It is worth noting that the addition of TiO2 reduced the transmittance of the blended film in the visible light region (800 nm) from 79.65% in P-40-25 to 2% in 5%-TiO2 nanocomposite, and the transmittance in the ultraviolet region (350 nm) reduced from 18.4% in P-40-25 to 0% in 5%-TiO2 nanocomposite. In addition, the transmittance varied significantly with the concentration of TiO2 . Similar results have been reported with the addition of TiO2 in starch [26,48], whey protein , and kefir–whey protein complex . The light transmittance of all the films is less (T < 1%) in the ultraviolet region (wavelengths below 300 nm), indicating that the blend film has good UV resistance. Therefore, the addition of MMT and TiO2 can improve the UV-barrier properties of the FK/PVA/Tris blend film.
complex . The light transmittance of all the films is less (T < 1%) in the ultraviolet region (wavelengths below 300 nm), indicating that the blend film has good UV resistance. Therefore, the addition of MMT and TiO2 can improve the UV‐barrier properties of the FK/PVA/Tris blend film. It can be seen from the transparency values in Figure 9 that the transparency value of the Nanomaterials nanocomposite 2019, 9,film 298 is higher than that of P‐40‐25, and the transparency value of the film increases 13 of 17 with increase in the content of nanoparticles. The specific transparency values of the blend films can be found Table in the Supplementary 3. Transmittance Materials (Table of the FK/PVA/Tris S2). At blend films the same modified withcontent differentof nanoparticles, contents of MMT andthe film containing TiO2 . TiO 2 exhibits higher transparency value than that containing MMT. The higher the transparency value, the lower is the transparency of the film and vice versa. Thus, the transparency of Sample P‐40‐25 is better than that of the nanocomposite %T blend film, and the transparency of MMT‐modified800FK/PVA/Trisnm 700 nm blend 600 nm film 500 nm is better 400 thannm that350ofnmTiO2300 nm ‐modified 280blend nm film. 200 nmThe transparency P-40-25 of79.65 a film is77.57 generally 74.21affected by additives, 66.73 41.49 processing 18.40 conditions, 0.67 0.10thickness, 0.00 and 0.5%-MMT between compatibility 74.10 the71.22 polymer67.10 59.56 and the nanoparticle 37.83[50–54]. 18.21 0.62 compatibility The limited 0.04 0.00 between 1%-MMT 68.55 65.65 61.95 54.25 32.92 18.05 0.53 0.00 0.00 the3%-MMT nanoparticles 67.60 and the matrix59.40 63.20 of FK/PVA/Tris, 51.20 especially16.40 27.30 with increase 0.38 in 0.00 the nanoparticle 0.00 content, 5%-MMT may result 62.30 in agglomeration 60.00 56.19of the 47.80 nanoparticles, 25.10 increasing 14.50 the0.20 internal scattering 0.00 of light 0.00 and0.5%-TiO the turbidity 2 56.15 51.81 . Therefore, 45.91 the 37.64 addition 21.95 of nanoparticles 11.46 0.10 on the0.00 has an effect 0.00 and appearance 1%-TiO2 41.00 35.30 27.80 20.50 9.20 3.80 0.10 0.00 0.00 the3%-TiO photoresistance 6.00 properties 3.70 of2.10the FK/PVA/Tris 1.30 0.50 blend 0.00 film, depending 0.00 on the type 0.00 0.00 of 2 nanoparticles 5%-TiO2 and 2.00the level of addition. 1.40 1.10 0.80 0.30 0.00 0.00 0.00 0.00 Table 3. Transmittance of the FK/PVA/Tris blend films modified with different contents of MMT It can be seen from the transparency values in Figure 9 that the transparency value of the and TiO2. nanocomposite film is higher than that of P-40-25, and the transparency value of the film increases with %T increase in the content of nanoparticles. The specific transparency values of the blend films can be found Sample Materials in the Supplementary 800 (Table 700 S2).600At the 500 400 of350 same content 300 280 nanoparticles, 200 containing the film nm value TiO2 exhibits higher transparency nm than nmthat containing nm nmMMT.nm nm the The higher nmtransparency nm value, the lower is theP‐40‐25 79.65of the transparency 77.57 film 74.21 and vice66.73 versa. 41.49 18.40 Thus, the 0.67 0.10 transparency 0.00 is better of P-40-25 than that of 0.5%‐MMT 74.10 blend the nanocomposite 71.22 film, 67.10and 59.56 37.83 18.21 the transparency 0.62 0.04 0.00 of MMT-modified FK/PVA/Tris blend film is1%‐MMT 68.55of TiO better than that 65.65 61.95 blend 2 -modified 54.25 film. 32.92 The18.05 0.53 0.00 transparency 0.00is generally of a film 3%‐MMTprocessing affected by additives, 67.60 conditions, 63.20 59.40thickness, 51.20 and27.30 16.40 0.38 compatibility 0.00 the between 0.00 polymer and 5%‐MMT the nanoparticle [50–54]. 62.30 60.00 compatibility The limited 56.19 47.80between25.10 the 14.50 0.20 0.00and0.00 nanoparticles the matrix of FK/PVA/Tris, 0.5%‐TiO especially 2 56.15 increase with 51.81 in45.91 37.64 21.95 the nanoparticle 11.46may0.10 content, result0.00 0.00 in agglomeration of 1%‐TiO the nanoparticles, 41.00the 35.30 increasing 2 internal27.80 20.50of light scattering 9.20 and3.80 0.10 0.00 the turbidity . 0.00 Therefore, the 3%‐TiO2 addition of nanoparticles 6.00an effect has 3.70 on2.10 1.30 the appearance 0.50 0.00 and the 0.00 0.00 properties photoresistance 0.00 of the FK/PVA/Tris5%‐TiO blend film, 2 2.00 depending 1.40on the 1.10 0.80 type of 0.30 nanoparticles 0.00 and the0.00 level 0.00 0.00 of addition. MMT TiO2 20 Transparency 15 10 5 0 1 2 3 4 5 Nanoparticle content (%) Figure 9. Transparency of the FK/PVA/Tris blend films modified with different contents of MMT and TiO2 . Nanomaterials 2019, 8, x; doi: FOR PEER REVIEW www.mdpi.com/journal/nanomaterials 4. Conclusions In this study, we successfully prepared FK/PVA/Tris nanocomposite films containing MMT or TiO2 . XRD studies showed that silicate platelets were exfoliated and TiO2 nanoparticles were uniformly dispersed in the film matrix. The shifting of the characteristic peaks of P-40-25, MMT,
Nanomaterials 2019, 9, 298 14 of 17 and TiO2 nanoparticles in the FTIR spectra indicated the formation of new hydrogen bonds in the nanocomposite matrix. It was observed that FK/PVA/Tris blend films containing MMT or TiO2 exhibited improved thermal, mechanical, and barrier properties compared with the unfilled material. Specifically, P-40-25 loaded with 3% of MMT exhibited maximum improvement in the properties: the elongation at break and the tensile strength increased by 133.06% and 9.29%, and the WVP and the OP decreased by 21.68% and 78.6% when compared to those of P-40-25. Meanwhile, P-40-25 loaded with 5% TiO2 exhibited maximum improvement in the properties: the elongation at break and the tensile strength increased by 434.6% and 36.95%, and the WVP and the OP decreased by 26.86% and 37.56% when compared to those of P-40-25. It is worth noting that the addition of MMT and TiO2 can improve the UV resistance of the films. Furthermore, the MMT nanocomposite films retained the visible transparency, while the TiO2 nanocomposite films increased the opacity. This study provides a method to improve the properties of keratin films for packaging applications. Supplementary Materials: The supplementary materials are available online at http://www.mdpi.com/2079- 4991/9/2/298/s1. Author Contributions: Conceptualization, X.C. and S.W.; Methodology, S.W. and M.H.; Software, S.W.; Validation, M.Y. and S.W.; Formal Analysis, S.W. and X.C.; Investigation, M.H. and J.G.; Resources, X.L.; Data Curation, J.G. and G.Y.; Writing—Original Draft Preparation, S.W.; Writing—Review and Editing, S.W. and X.C.; Supervision, G.Y.; Project Administration, X.C.; Funding Acquisition, X.L. Funding: This research was supported by the National Natural Science Foundation of Guangdong Province (2016A030313371) and the Science and Technology Plan Project of Guangzhou (201704030130). Acknowledgments: The authors also like to thank Editage [www.editage.cn] for English language editing. Conflicts of Interest: The authors declare no conflicts of interest. References 1. Abdorreza, M.N.; Cheng, L.; Karim, A. Effects of plasticizers on thermal properties and heat sealability of sago starch films. Food Hydrocoll. 2011, 25, 56–60. [CrossRef] 2. Jang, S.A.; Shin, Y.J.; Song, K.B. Effect of rapeseed protein–gelatin film containing grapefruit seed extract on ‘maehyang’ strawberry quality. Int. J. Food Sci. Technol. 2011, 46, 620–625. [CrossRef] 3. Jin, E.; Reddy, N.; Zhu, Z.; Yang, Y. Graft polymerization of native chicken feathers for thermoplastic applications. J. Agric. Food Chem. 2011, 59, 1729–1738. [CrossRef] [PubMed] 4. Zhao, L.; Zhou, H.; Hua, J. New progress in utilization of feather fibers. China Leather 2011, 40, 36–40. 5. Zhang, Y.Q. Dissociation and Extraction of Feather Keratin by Steam Flash Explosion. Ph.D. Thesis, Jiangnan University, Wuxi, China, 2016. 6. Brown, E.M.; Pandya, K.; Taylor, M.M.; Liu, C.-K. Comparison of methods for extraction of keratin from waste wool. Agric. Sci. 2016, 7, 670–679. [CrossRef] 7. Shavandi, A.; Bekhit, A.E.; Carne, A.; Bekhit, A. Evaluation of keratin extraction from wool by chemical methods for bio-polymer application. J. Bioact. Compat. Polym. 2016, 32, 163–177. [CrossRef] 8. Jiang, S.Q.; Zhang, L.; Wu, H.X.; Chi, G. Study on effective extraction of keratin from human hair wastes. Integr. Ferroelectr. 2017, 180, 102–107. 9. Kang, D.; Herschend, J.; Al-Soud, W.A.; Mortensen, M.S.; Gonzalo, M.; Jacquiod, S.; Sørensen, S.J. Enrichment and characterization of an environmental microbial consortium displaying efficient keratinolytic activity. Bioresour. Technol. 2018, 270, 303–310. [CrossRef] [PubMed] 10. Sekar, V.; Kannan, M.; Ganesan, R.; Dheeba, B.; Sivakumar, N.; Kannan, K. Isolation and screening of keratinolytic bacteria from feather dumping soil in and around Cuddalore and Villupuram, Tamil Nadu. Proc. Natl. Acad. Sci. India 2015, 86, 1–9. [CrossRef] 11. Dou, Y.; Huang, X.; Zhang, B.; He, M.; Yin, G.; Cui, Y. Preparation and characterization of dialdehyde starch crosslinked feather keratin film for food packaging application. RSC Adv. 2015, 5, 27168–27174. [CrossRef] 12. Dou, Y.; Zhang, B.; He, M.; Yin, G.; Cui, Y.; Savina, I.N. Keratin/polyvinyl alcohol blend films cross-linked by dialdehyde starch and their potential application for drug release. Polymers 2015, 7, 580–591. [CrossRef] 13. He, M.; Zhang, B.; Dou, Y.; Yin, G.; Cui, Y. Blend modification of feather keratin-based films using sodium alginate. J. Appl. Polym. Sci. 2017, 134, 44680–44687. [CrossRef]
You can also read
Next slide ... Cancel